#------------------------------------------------------------------------------
#$Date: 2016-03-25 15:35:39 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179926 $
#$URL: svn://www.crystallography.net/cod/cif/7/02/21/7022170.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7022170
loop_
_publ_author_name
'Sha, Jing-Quan'
'Sun, Jing-Wen'
'Li, Meng-Ting'
'Wang, Cheng'
'Li, Guang-Ming'
'Yan, Peng-Fei'
'Sun, Long-Jiang'
_publ_section_title
;
 Secondary spacer modulated assembly of polyoxometalate based
 metal-organic frameworks.
;
_journal_issue                   5
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1667
_journal_page_last               1677
_journal_paper_doi               10.1039/c2dt31951a
_journal_volume                  42
_journal_year                    2013
_chemical_formula_moiety
'C36 H28 Cu5 Mo12 N30 O44 Si,2(H2O), 2(H O0.50) '
_chemical_formula_sum            'C36 H34 Cu5 Mo12 N30 O47 Si'
_chemical_formula_weight         3136.05
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                105.129(5)
_cell_angle_beta                 111.458(5)
_cell_angle_gamma                105.677(5)
_cell_formula_units_Z            1
_cell_length_a                   12.168(5)
_cell_length_b                   13.460(5)
_cell_length_c                   14.191(5)
_cell_measurement_reflns_used    1512
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      22.1702
_cell_measurement_theta_min      2.4727
_cell_volume                     1907.3(13)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0328
_diffrn_reflns_av_sigmaI/netI    0.0836
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9621
_diffrn_reflns_theta_full        24.99
_diffrn_reflns_theta_max         24.99
_diffrn_reflns_theta_min         1.68
_exptl_absorpt_coefficient_mu    3.395
_exptl_absorpt_correction_T_max  0.643
_exptl_absorpt_correction_T_min  0.429
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs(Sheldrick,1996)
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.730
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       strip
_exptl_crystal_F_000             1499
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.13
_refine_diff_density_max         1.380
_refine_diff_density_min         -1.762
_refine_diff_density_rms         0.200
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     617
_refine_ls_number_reflns         6708
_refine_ls_number_restraints     72
_refine_ls_restrained_S_all      1.056
_refine_ls_R_factor_all          0.1211
_refine_ls_R_factor_gt           0.0749
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0309P)²+49.9430P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1458
_refine_ls_wR_factor_ref         0.1689
_reflns_number_gt                4249
_reflns_number_total             6708
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt31951a.txt
_cod_data_source_block           dd
_cod_database_code               7022170
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.69714(13) 0.30490(11) 0.27618(11) 0.0373(3) Uani 1 1 d .
Mo2 Mo 0.84084(14) 0.24317(13) 0.50679(14) 0.0586(5) Uani 1 1 d .
Mo3 Mo 0.97727(18) 0.35491(12) 0.24366(12) 0.0538(5) Uani 1 1 d .
Mo4 Mo 0.85446(15) 0.56535(13) 0.27239(11) 0.0429(4) Uani 1 1 d .
Mo5 Mo 1.28174(15) 0.54847(17) 0.46758(14) 0.0699(6) Uani 1 1 d .
Mo6 Mo 1.1189(2) 0.29129(17) 0.46914(15) 0.0805(7) Uani 1 1 d .
Cu1 Cu 0.64910(16) 0.55598(13) -0.03295(15) 0.0286(4) Uani 1 1 d .
Cu2 Cu 1.0000 1.0000 0.0000 0.0412(7) Uani 1 2 d S
Cu3 Cu 0.53221(16) 0.95192(15) 0.12723(15) 0.0324(4) Uani 1 1 d .
Si1 Si 1.0000 0.5000 0.5000 0.0280(12) Uani 1 2 d S
O1 O 0.8077(15) 0.2742(12) 0.2204(13) 0.084(4) Uani 1 1 d U
O1W O 0.4974(11) 0.4868(11) -0.2306(10) 0.066(4) Uani 1 1 d .
H105 H 0.5082 0.5319 -0.2618 0.079 Uiso 1 1 d R
H106 H 0.4228 0.4716 -0.2347 0.079 Uiso 1 1 d R
O2 O 0.9583(12) 0.2076(14) 0.4639(10) 0.094(6) Uani 1 1 d .
O2W O 0.4890(11) 0.9889(11) 0.2526(9) 0.056(3) Uani 1 1 d .
O3 O 1.1790(14) 0.1949(11) 0.4594(11) 0.072(4) Uani 1 1 d .
O4 O 0.7863(10) 0.5932(9) 0.1644(9) 0.050(3) Uani 1 1 d .
O5 O 0.8096(11) 0.6425(13) 0.3722(10) 0.082(5) Uani 1 1 d .
O6 O 0.6464(12) 0.3743(11) 0.3815(9) 0.059(3) Uani 1 1 d .
O7 O 0.7366(12) 0.2172(11) 0.3616(9) 0.064(4) Uani 1 1 d .
O8 O 0.7574(13) 0.3300(12) 0.5538(10) 0.073(4) Uani 1 1 d .
O9 O 0.5543(11) 0.2098(9) 0.1755(9) 0.061(4) Uani 1 1 d .
O10 O 1.4122(13) 0.5728(15) 0.4516(12) 0.097(5) Uani 1 1 d .
O11 O 0.9795(11) 0.3206(14) 0.6563(10) 0.088(5) Uani 1 1 d .
O12 O 1.2636(17) 0.4123(14) 0.4871(14) 0.117(6) Uani 1 1 d U
O13 O 0.7672(15) 0.1251(12) 0.5134(12) 0.092(5) Uani 1 1 d U
O14 O 1.0269(16) 0.2652(12) 0.3216(12) 0.104(5) Uani 1 1 d U
O15 O 0.7108(14) 0.4295(11) 0.2362(13) 0.078(4) Uani 1 1 d U
O17 O 1.0790(17) 0.4423(15) 0.4418(14) 0.028(4) Uani 0.50 1 d P
O18 O 0.8705(16) 0.4058(14) 0.4662(15) 0.027(4) Uani 0.50 1 d PU
O19 O 0.8992(16) 0.4444(14) 0.3638(14) 0.023(4) Uani 0.50 1 d P
O20 O 1.0135(16) 0.4003(14) 0.5397(15) 0.025(4) Uani 0.50 1 d P
O21 O 1.1520(16) 0.4593(13) 0.3183(13) 0.109(6) Uani 1 1 d U
O22 O 0.9197(15) 0.4662(12) 0.2128(14) 0.090(4) Uani 1 1 d U
O23 O 0.9698(10) 0.2918(9) 0.1241(9) 0.047(3) Uani 1 1 d .
N1 N 0.8615(12) 0.9614(10) -0.1517(10) 0.035(3) Uani 1 1 d .
N2 N 0.8859(12) 0.8462(9) -0.0265(10) 0.034(3) Uani 1 1 d .
N3 N 0.8646(13) 0.7742(11) 0.0218(11) 0.046(3) Uani 1 1 d .
N4 N 0.7562(12) 0.6902(10) -0.0461(10) 0.033(3) Uani 1 1 d .
N5 N 0.6985(12) 0.6974(10) -0.1452(11) 0.041(3) Uani 1 1 d .
N8 N 1.3647(10) 0.9877(9) -0.0589(9) 0.028(3) Uani 1 1 d .
N9 N 1.2972(11) 1.0440(10) -0.2253(9) 0.032(3) Uani 1 1 d .
N11 N 0.5659(10) 0.7389(8) 0.0251(9) 0.024(2) Uani 1 1 d .
N12 N 0.4770(10) 0.7617(9) 0.0540(9) 0.026(3) Uani 1 1 d .
N13 N 1.3758(11) 0.9594(9) 0.0267(9) 0.031(3) Uani 1 1 d .
N14 N 1.2659(11) 0.9387(10) 0.0339(10) 0.036(3) Uani 1 1 d .
N15 N 1.1822(11) 0.9554(10) -0.0464(10) 0.034(3) Uani 1 1 d .
N17 N 0.5491(11) 0.6351(9) 0.0136(9) 0.026(3) Uani 1 1 d .
C1 C 0.7664(14) 0.8570(13) -0.2001(12) 0.037(4) Uani 1 1 d .
C2 C 0.7821(14) 0.7959(11) -0.1286(12) 0.032(3) Uani 1 1 d .
C3 C 0.6606(14) 0.8109(15) -0.3066(13) 0.047(4) Uani 1 1 d .
H3 H 0.5982 0.7376 -0.3388 0.056 Uiso 1 1 calc R
C4 C 0.6578(19) 0.8832(18) -0.3583(16) 0.065(5) Uani 1 1 d .
H4 H 0.5890 0.8585 -0.4282 0.078 Uiso 1 1 calc R
C5 C 0.7553(18) 0.9951(16) -0.3107(15) 0.054(5) Uani 1 1 d .
H5 H 0.7516 1.0418 -0.3488 0.065 Uiso 1 1 calc R
C6 C 0.8557(16) 1.0312(15) -0.2052(14) 0.045(4) Uani 1 1 d .
H6 H 0.9195 1.1041 -0.1709 0.054 Uiso 1 1 calc R
C13 C 1.2067(13) 1.0129(11) -0.1983(11) 0.030(3) Uani 1 1 d .
C14 C 1.0864(17) 1.0104(15) -0.2538(14) 0.054(5) Uani 1 1 d .
H14 H 1.0200 0.9806 -0.2382 0.065 Uiso 1 1 calc R
C15 C 1.1615(17) 1.0878(15) -0.3615(14) 0.055(5) Uani 1 1 d .
H15 H 1.1499 1.1158 -0.4162 0.066 Uiso 1 1 calc R
C16 C 1.2466(13) 0.9831(11) -0.1029(12) 0.030(3) Uani 1 1 d .
C17 C 1.0671(18) 1.0551(17) -0.3358(14) 0.059(5) Uani 1 1 d .
H17 H 0.9896 1.0613 -0.3710 0.070 Uiso 1 1 calc R
C18 C 1.2747(18) 1.0803(15) -0.3079(14) 0.056(5) Uani 1 1 d .
H18 H 1.3388 1.1008 -0.3286 0.067 Uiso 1 1 calc R
N6 N 0.4485(10) 0.5874(9) 0.0283(9) 0.023(2) Uani 1 1 d .
C7 C 0.4067(12) 0.6682(11) 0.0531(10) 0.023(3) Uani 1 1 d .
C8 C 0.3000(13) 0.6433(11) 0.0795(12) 0.027(3) Uani 1 1 d U
C12 C 0.2420(14) 0.7143(12) 0.1019(14) 0.039(4) Uani 1 1 d U
H12 H 0.2673 0.7841 0.0979 0.047 Uiso 1 1 calc R
N10 N 0.2616(11) 0.5379(9) 0.0795(10) 0.035(3) Uani 1 1 d U
C9 C 0.1483(18) 0.6814(15) 0.1298(17) 0.062(6) Uani 1 1 d U
H9 H 0.1048 0.7269 0.1409 0.074 Uiso 1 1 calc R
C11 C 0.1727(17) 0.5103(15) 0.1103(17) 0.057(5) Uani 1 1 d U
H11 H 0.1455 0.4391 0.1112 0.069 Uiso 1 1 calc R
C10 C 0.116(2) 0.5820(16) 0.1421(18) 0.068(6) Uani 1 1 d U
H10 H 0.0590 0.5627 0.1702 0.082 Uiso 1 1 calc R
O3W O 0.4569(19) 0.8873(17) 0.3866(16) 0.141(7) Uani 1 1 d U
H104 H 0.4670 0.9187 0.3436 0.169 Uiso 1 1 d R
H103 H 0.3787 0.8452 0.3588 0.169 Uiso 1 1 d R
O4W O 1.463(2) 1.275(2) -0.358(2) 0.064(7) Uani 0.50 1 d PU
H101 H 1.5236 1.3313 -0.3002 0.076 Uiso 0.50 1 d PR
H102 H 1.3970 1.2897 -0.3791 0.076 Uiso 0.50 1 d PR
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O9 Mo1 O1 101.7(7) . .
O9 Mo1 O15 101.4(6) . .
O1 Mo1 O15 90.0(6) . .
O9 Mo1 O7 98.2(6) . .
O1 Mo1 O7 88.6(6) . .
O15 Mo1 O7 160.2(6) . .
O9 Mo1 O6 100.0(6) . .
O1 Mo1 O6 158.1(6) . .
O15 Mo1 O6 88.1(5) . .
O7 Mo1 O6 85.9(5) . .
O9 Mo1 O19 160.1(6) . .
O1 Mo1 O19 65.6(6) . .
O15 Mo1 O19 64.9(6) . .
O7 Mo1 O19 96.7(6) . .
O6 Mo1 O19 94.1(6) . .
O9 Mo1 O18 155.5(6) . .
O1 Mo1 O18 93.3(7) . .
O15 Mo1 O18 97.8(6) . .
O7 Mo1 O18 62.6(6) . .
O6 Mo1 O18 65.4(5) . .
O19 Mo1 O18 44.3(6) . .
O13 Mo2 O7 101.5(7) . .
O13 Mo2 O2 100.6(8) . .
O7 Mo2 O2 89.0(6) . .
O13 Mo2 O8 99.9(8) . .
O7 Mo2 O8 89.3(5) . .
O2 Mo2 O8 159.3(7) . .
O13 Mo2 O11 99.1(7) . .
O7 Mo2 O11 159.4(7) . .
O2 Mo2 O11 87.9(5) . .
O8 Mo2 O11 86.5(5) . .
O13 Mo2 O20 157.8(7) . .
O7 Mo2 O20 96.1(6) . .
O2 Mo2 O20 66.0(7) . .
O8 Mo2 O20 93.7(6) . .
O11 Mo2 O20 64.1(7) . .
O13 Mo2 O18 159.8(7) . .
O7 Mo2 O18 64.8(6) . .
O2 Mo2 O18 94.2(7) . .
O8 Mo2 O18 66.5(6) . .
O11 Mo2 O18 95.2(7) . .
O20 Mo2 O18 42.4(6) . .
O23 Mo3 O21 98.3(7) . .
O23 Mo3 O22 98.7(6) . .
O21 Mo3 O22 91.4(7) . .
O23 Mo3 O14 102.4(7) . .
O21 Mo3 O14 89.1(6) . .
O22 Mo3 O14 158.6(7) . .
O23 Mo3 O1 102.4(6) . .
O21 Mo3 O1 159.2(7) . .
O22 Mo3 O1 87.1(6) . .
O14 Mo3 O1 85.0(7) . .
O23 Mo3 O17 154.6(6) . .
O21 Mo3 O17 62.5(7) . .
O22 Mo3 O17 98.3(6) . .
O14 Mo3 O17 63.1(6) . .
O1 Mo3 O17 97.1(6) . .
O23 Mo3 O19 154.7(6) . .
O21 Mo3 O19 99.6(7) . .
O22 Mo3 O19 63.3(6) . .
O14 Mo3 O19 95.6(7) . .
O1 Mo3 O19 61.4(6) . .
O17 Mo3 O19 50.6(6) . .
O4 Mo4 O11 100.4(6) . 2_766
O4 Mo4 O5 102.0(6) . .
O11 Mo4 O5 91.7(5) 2_766 .
O4 Mo4 O22 99.3(7) . .
O11 Mo4 O22 88.1(6) 2_766 .
O5 Mo4 O22 158.4(7) . .
O4 Mo4 O15 98.9(6) . .
O11 Mo4 O15 160.4(7) 2_766 .
O5 Mo4 O15 87.4(6) . .
O22 Mo4 O15 85.7(6) . .
O4 Mo4 O19 154.5(6) . .
O11 Mo4 O19 98.7(7) 2_766 .
O5 Mo4 O19 94.1(7) . .
O22 Mo4 O19 64.6(6) . .
O15 Mo4 O19 61.9(6) . .
O4 Mo4 O20 158.6(6) . 2_766
O11 Mo4 O20 63.7(6) 2_766 2_766
O5 Mo4 O20 66.2(6) . 2_766
O22 Mo4 O20 94.6(7) . 2_766
O15 Mo4 O20 98.3(6) . 2_766
O19 Mo4 O20 46.9(6) . 2_766
O10 Mo5 O6 100.9(7) . 2_766
O10 Mo5 O8 100.2(8) . 2_766
O6 Mo5 O8 89.7(5) 2_766 2_766
O10 Mo5 O12 99.6(9) . .
O6 Mo5 O12 89.6(7) 2_766 .
O8 Mo5 O12 159.9(8) 2_766 .
O10 Mo5 O21 100.2(8) . .
O6 Mo5 O21 158.9(7) 2_766 .
O8 Mo5 O21 86.2(6) 2_766 .
O12 Mo5 O21 87.3(6) . .
O10 Mo5 O17 156.7(8) . .
O6 Mo5 O17 96.0(6) 2_766 .
O8 Mo5 O17 95.8(6) 2_766 .
O12 Mo5 O17 64.4(7) . .
O21 Mo5 O17 63.9(7) . .
O10 Mo5 O18 157.2(8) . 2_766
O6 Mo5 O18 64.9(5) 2_766 2_766
O8 Mo5 O18 63.6(6) 2_766 2_766
O12 Mo5 O18 98.1(7) . 2_766
O21 Mo5 O18 94.8(7) . 2_766
O17 Mo5 O18 46.1(6) . 2_766
O3 Mo6 O14 101.6(7) . .
O3 Mo6 O5 98.5(6) . 2_766
O14 Mo6 O5 160.0(7) . 2_766
O3 Mo6 O12 97.2(8) . .
O14 Mo6 O12 90.8(6) . .
O5 Mo6 O12 86.9(7) 2_766 .
O3 Mo6 O2 100.2(7) . .
O14 Mo6 O2 89.0(7) . .
O5 Mo6 O2 87.3(5) 2_766 .
O12 Mo6 O2 162.3(7) . .
O3 Mo6 O17 156.2(6) . .
O14 Mo6 O17 65.8(6) . .
O5 Mo6 O17 95.5(6) 2_766 .
O12 Mo6 O17 64.3(7) . .
O2 Mo6 O17 99.7(7) . .
O3 Mo6 O20 154.8(6) . .
O14 Mo6 O20 96.7(7) . .
O5 Mo6 O20 64.2(6) 2_766 .
O12 Mo6 O20 99.7(7) . .
O2 Mo6 O20 62.8(6) . .
O17 Mo6 O20 48.7(6) . .
N17 Cu1 N6 93.3(4) . 2_665
N17 Cu1 N10 174.1(4) . 2_665
N6 Cu1 N10 80.8(4) 2_665 2_665
N17 Cu1 N4 93.2(4) . .
N6 Cu1 N4 173.4(5) 2_665 .
N10 Cu1 N4 92.7(4) 2_665 .
N2 Cu2 N2 180.000(2) 2_775 .
N2 Cu2 N1 82.2(5) 2_775 2_775
N2 Cu2 N1 97.8(5) . 2_775
N2 Cu2 N1 97.8(5) 2_775 .
N2 Cu2 N1 82.2(5) . .
N1 Cu2 N1 180.000(2) 2_775 .
N13 Cu3 N8 93.4(4) 1_455 2_775
N13 Cu3 N9 173.8(5) 1_455 2_775
N8 Cu3 N9 80.7(5) 2_775 2_775
N13 Cu3 O2W 91.6(5) 1_455 .
N8 Cu3 O2W 145.5(5) 2_775 .
N9 Cu3 O2W 92.1(5) 2_775 .
N13 Cu3 N12 100.2(4) 1_455 .
N8 Cu3 N12 103.9(4) 2_775 .
N9 Cu3 N12 83.3(4) 2_775 .
O2W Cu3 N12 108.8(5) . .
O18 Si1 O18 180(2) 2_766 .
O18 Si1 O20 65.5(8) 2_766 2_766
O18 Si1 O20 114.5(8) . 2_766
O18 Si1 O20 114.5(8) 2_766 .
O18 Si1 O20 65.5(8) . .
O20 Si1 O20 180.0(13) 2_766 .
O18 Si1 O19 112.9(8) 2_766 .
O18 Si1 O19 67.1(8) . .
O20 Si1 O19 70.6(8) 2_766 .
O20 Si1 O19 109.4(8) . .
O18 Si1 O19 67.1(8) 2_766 2_766
O18 Si1 O19 112.9(8) . 2_766
O20 Si1 O19 109.4(8) 2_766 2_766
O20 Si1 O19 70.6(8) . 2_766
O19 Si1 O19 180.000(5) . 2_766
O18 Si1 O17 108.2(9) 2_766 2_766
O18 Si1 O17 71.8(9) . 2_766
O20 Si1 O17 73.0(8) 2_766 2_766
O20 Si1 O17 107.0(8) . 2_766
O19 Si1 O17 104.1(8) . 2_766
O19 Si1 O17 75.9(8) 2_766 2_766
O18 Si1 O17 71.8(9) 2_766 .
O18 Si1 O17 108.2(9) . .
O20 Si1 O17 107.0(8) 2_766 .
O20 Si1 O17 73.0(8) . .
O19 Si1 O17 75.9(8) . .
O19 Si1 O17 104.1(8) 2_766 .
O17 Si1 O17 180.000(6) 2_766 .
Mo1 O1 Mo3 136.5(8) . .
H105 O1W H106 107.7 . .
Mo2 O2 Mo6 136.1(9) . .
Mo4 O5 Mo6 135.9(7) . 2_766
Mo5 O6 Mo1 138.2(6) 2_766 .
Mo2 O7 Mo1 137.8(8) . .
Mo5 O8 Mo2 136.8(8) 2_766 .
Mo4 O11 Mo2 135.6(9) 2_766 .
Mo5 O12 Mo6 133.0(10) . .
Mo6 O14 Mo3 135.2(9) . .
Mo1 O15 Mo4 134.2(8) . .
Si1 O17 Mo6 120.9(9) . .
Si1 O17 Mo5 122.3(9) . .
Mo6 O17 Mo5 98.2(7) . .
Si1 O17 Mo3 117.6(8) . .
Mo6 O17 Mo3 95.4(6) . .
Mo5 O17 Mo3 96.6(6) . .
Si1 O18 O20 59.3(8) . .
Si1 O18 O19 60.2(8) . .
O20 O18 O19 100.6(12) . .
Si1 O18 Mo2 126.9(9) . .
O20 O18 Mo2 67.7(8) . .
O19 O18 Mo2 135.5(11) . .
Si1 O18 Mo1 123.1(9) . .
O20 O18 Mo1 135.1(11) . .
O19 O18 Mo1 62.9(8) . .
Mo2 O18 Mo1 94.4(6) . .
Si1 O18 Mo5 119.9(9) . 2_766
O20 O18 Mo5 128.5(11) . 2_766
O19 O18 Mo5 123.9(10) . 2_766
Mo2 O18 Mo5 92.1(6) . 2_766
Mo1 O18 Mo5 91.2(6) . 2_766
Si1 O19 O18 52.8(7) . .
Si1 O19 Mo1 125.5(8) . .
O18 O19 Mo1 72.8(8) . .
Si1 O19 Mo4 119.7(8) . .
O18 O19 Mo4 137.5(11) . .
Mo1 O19 Mo4 98.7(6) . .
Si1 O19 Mo3 115.9(8) . .
O18 O19 Mo3 127.7(10) . .
Mo1 O19 Mo3 96.2(6) . .
Mo4 O19 Mo3 94.3(6) . .
Si1 O20 O18 55.3(7) . .
Si1 O20 Mo2 125.2(9) . .
O18 O20 Mo2 69.9(8) . .
Si1 O20 Mo4 122.7(9) . 2_766
O18 O20 Mo4 136.8(11) . 2_766
Mo2 O20 Mo4 95.8(6) . 2_766
Si1 O20 Mo6 117.3(9) . .
O18 O20 Mo6 127.5(11) . .
Mo2 O20 Mo6 95.1(6) . .
Mo4 O20 Mo6 93.3(5) 2_766 .
Mo3 O21 Mo5 137.0(10) . .
Mo4 O22 Mo3 137.8(9) . .
C1 N1 C6 119.5(14) . .
C1 N1 Cu2 114.9(9) . .
C6 N1 Cu2 125.6(11) . .
N3 N2 C2 104.4(11) . .
N3 N2 Cu2 144.1(10) . .
C2 N2 Cu2 111.2(9) . .
N4 N3 N2 108.6(12) . .
N3 N4 N5 112.7(11) . .
N3 N4 Cu1 133.2(10) . .
N5 N4 Cu1 114.0(9) . .
C2 N5 N4 101.8(12) . .
C16 N8 N13 104.7(11) . .
C16 N8 Cu3 113.0(9) . 2_775
N13 N8 Cu3 141.8(9) . 2_775
C13 N9 C18 119.0(13) . .
C13 N9 Cu3 115.3(9) . 2_775
C18 N9 Cu3 125.4(11) . 2_775
N17 N11 N12 107.4(10) . .
C7 N12 N11 106.1(10) . .
C7 N12 Cu3 140.2(9) . .
N11 N12 Cu3 111.1(7) . .
N14 N13 N8 110.0(10) . .
N14 N13 Cu3 125.6(9) . 1_655
N8 N13 Cu3 124.4(9) . 1_655
N13 N14 N15 108.8(11) . .
N14 N15 C16 104.0(11) . .
N11 N17 N6 110.2(10) . .
N11 N17 Cu1 124.6(9) . .
N6 N17 Cu1 125.0(8) . .
N1 C1 C3 125.0(15) . .
N1 C1 C2 112.6(12) . .
C3 C1 C2 122.4(14) . .
N5 C2 N2 112.6(13) . .
N5 C2 C1 127.9(13) . .
N2 C2 C1 119.1(12) . .
C4 C3 C1 114.1(16) . .
C4 C3 H3 123.0 . .
C1 C3 H3 123.0 . .
C3 C4 C5 123.4(17) . .
C3 C4 H4 118.3 . .
C5 C4 H4 118.3 . .
C6 C5 C4 117.3(15) . .
C6 C5 H5 121.3 . .
C4 C5 H5 121.3 . .
N1 C6 C5 120.7(16) . .
N1 C6 H6 119.7 . .
C5 C6 H6 119.7 . .
N9 C13 C14 122.6(14) . .
N9 C13 C16 113.4(12) . .
C14 C13 C16 124.0(14) . .
C13 C14 C17 117.5(17) . .
C13 C14 H14 121.3 . .
C17 C14 H14 121.3 . .
C17 C15 C18 119.9(16) . .
C17 C15 H15 120.1 . .
C18 C15 H15 120.1 . .
N8 C16 N15 112.5(12) . .
N8 C16 C13 117.4(13) . .
N15 C16 C13 130.1(12) . .
C15 C17 C14 118.9(16) . .
C15 C17 H17 120.6 . .
C14 C17 H17 120.6 . .
N9 C18 C15 121.9(17) . .
N9 C18 H18 119.0 . .
C15 C18 H18 119.0 . .
N17 N6 C7 105.1(9) . .
N17 N6 Cu1 141.5(8) . 2_665
C7 N6 Cu1 113.4(8) . 2_665
N12 C7 N6 111.1(11) . .
N12 C7 C8 130.6(12) . .
N6 C7 C8 118.2(11) . .
N10 C8 C12 122.3(12) . .
N10 C8 C7 112.0(11) . .
C12 C8 C7 125.7(12) . .
C9 C12 C8 118.9(13) . .
C9 C12 H12 120.5 . .
C8 C12 H12 120.5 . .
C11 N10 C8 116.8(13) . .
C11 N10 Cu1 127.7(10) . 2_665
C8 N10 Cu1 115.5(9) . 2_665
C12 C9 C10 120.8(15) . .
C12 C9 H9 119.6 . .
C10 C9 H9 119.6 . .
N10 C11 C10 123.7(15) . .
N10 C11 H11 118.1 . .
C10 C11 H11 118.1 . .
C9 C10 C11 116.8(15) . .
C9 C10 H10 121.6 . .
C11 C10 H10 121.6 . .
H104 O3W H103 108.8 . .
H101 O4W H102 108.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O9 1.651(10) .
Mo1 O1 1.875(13) .
Mo1 O15 1.891(13) .
Mo1 O7 1.929(11) .
Mo1 O6 1.935(11) .
Mo1 O19 2.273(16) .
Mo1 O18 2.438(17) .
Mo2 O13 1.645(12) .
Mo2 O7 1.857(10) .
Mo2 O2 1.870(12) .
Mo2 O8 1.890(12) .
Mo2 O11 1.927(12) .
Mo2 O20 2.338(17) .
Mo2 O18 2.374(17) .
Mo3 O23 1.644(10) .
Mo3 O21 1.892(16) .
Mo3 O22 1.900(14) .
Mo3 O14 1.910(13) .
Mo3 O1 1.910(14) .
Mo3 O17 2.400(17) .
Mo3 O19 2.447(17) .
Mo4 O4 1.648(9) .
Mo4 O11 1.865(13) 2_766
Mo4 O5 1.867(11) .
Mo4 O22 1.898(14) .
Mo4 O15 1.947(13) .
Mo4 O19 2.386(16) .
Mo4 O20 2.393(17) 2_766
Mo5 O10 1.643(12) .
Mo5 O6 1.846(11) 2_766
Mo5 O8 1.890(13) 2_766
Mo5 O12 1.892(14) .
Mo5 O21 1.903(16) .
Mo5 O17 2.328(19) .
Mo5 O18 2.505(18) 2_766
Mo6 O3 1.652(11) .
Mo6 O14 1.858(14) .
Mo6 O5 1.929(12) 2_766
Mo6 O12 1.929(17) .
Mo6 O2 1.938(15) .
Mo6 O17 2.308(17) .
Mo6 O20 2.448(17) .
Cu1 N17 1.992(11) .
Cu1 N6 2.006(10) 2_665
Cu1 N10 2.011(12) 2_665
Cu1 N4 2.019(11) .
Cu2 N2 2.003(11) 2_775
Cu2 N2 2.003(11) .
Cu2 N1 2.008(12) 2_775
Cu2 N1 2.008(12) .
Cu3 N13 1.965(11) 1_455
Cu3 N8 1.980(11) 2_775
Cu3 N9 2.008(11) 2_775
Cu3 O2W 2.013(11) .
Cu3 N12 2.293(10) .
Si1 O18 1.540(17) 2_766
Si1 O18 1.540(17) .
Si1 O20 1.610(16) 2_766
Si1 O20 1.610(16) .
Si1 O19 1.678(17) .
Si1 O19 1.678(17) 2_766
Si1 O17 1.691(18) 2_766
Si1 O17 1.691(18) .
O1W H105 0.8500 .
O1W H106 0.8500 .
O5 Mo6 1.929(12) 2_766
O6 Mo5 1.846(11) 2_766
O8 Mo5 1.890(13) 2_766
O11 Mo4 1.865(13) 2_766
O18 O20 1.70(2) .
O18 O19 1.78(2) .
O18 Mo5 2.505(18) 2_766
O20 Mo4 2.393(17) 2_766
N1 C1 1.349(18) .
N1 C6 1.354(17) .
N2 N3 1.348(16) .
N2 C2 1.356(18) .
N3 N4 1.281(17) .
N4 N5 1.366(16) .
N5 C2 1.334(17) .
N8 C16 1.317(16) .
N8 N13 1.338(15) .
N8 Cu3 1.980(11) 2_775
N9 C13 1.294(17) .
N9 C18 1.352(19) .
N9 Cu3 2.008(11) 2_775
N11 N17 1.313(14) .
N11 N12 1.367(14) .
N12 C7 1.310(15) .
N13 N14 1.338(15) .
N13 Cu3 1.965(11) 1_655
N14 N15 1.340(15) .
N15 C16 1.361(18) .
N17 N6 1.338(14) .
C1 C3 1.41(2) .
C1 C2 1.46(2) .
C3 C4 1.36(2) .
C3 H3 0.9300 .
C4 C5 1.43(3) .
C4 H4 0.9300 .
C5 C6 1.39(2) .
C5 H5 0.9300 .
C6 H6 0.9300 .
C13 C14 1.37(2) .
C13 C16 1.462(18) .
C14 C17 1.42(2) .
C14 H14 0.9300 .
C15 C17 1.33(2) .
C15 C18 1.35(2) .
C15 H15 0.9300 .
C17 H17 0.9300 .
C18 H18 0.9300 .
N6 C7 1.340(16) .
N6 Cu1 2.006(10) 2_665
C7 C8 1.457(17) .
C8 N10 1.369(15) .
C8 C12 1.372(18) .
C12 C9 1.34(2) .
C12 H12 0.9300 .
N10 C11 1.309(19) .
N10 Cu1 2.011(12) 2_665
C9 C10 1.36(2) .
C9 H9 0.9300 .
C11 C10 1.41(2) .
C11 H11 0.9300 .
C10 H10 0.9300 .
O3W H104 0.8521 .
O3W H103 0.8359 .
O4W H101 0.8508 .
O4W H102 0.8383 .
